Current State of Nanofiber Produced by Electrospinning and ... and mass production of nanofiber...
Embed Size (px)
Transcript of Current State of Nanofiber Produced by Electrospinning and ... and mass production of nanofiber...
Journal of Textile Engineering (2008), Vol.54, No.6, 199 - 205
© 2008 The Textile Machinery Society of Japan
Current State of Nanofiber Produced by Electrospinning and Prospects
for Mass Production
Materials Science, The University of Shiga Prefecture,
2500 Hassaka, Hikone, Shiga 522−8533, Japan
Received 20 October 2008; accepted for publication 7 November 2008
Abstract Melt electrospinning was able to achieve a thin fiber with nano-order diameter by controlling the amount of
discharge. Biomaterial is one of the fields where nanofiber is actively studied. The challenge of Japan for application and mass production of nanofiber noticed at present is also explained in this paper. Hirose paper Co. Ltd. proposed the production technique for an electrospinning in bubbles which continuously arise in polymer solution by applying high voltage. In NEDO project of Japan, the productivity was improved by increasing number of nozzle and became 50 times as great as the previous one. In Shiga Prefecture, the manufacturing equipment was also developed.
Key Words: Electrospinning, Nanofiber, Multi nozzle, Melt electrospinning
Nanofiber produced through an electrospinning process is widely utilized in medical filters, electronic materials, etc. . Moreover, manufacture of electrospinning machines of a solution-spun type has started in Japan as well. This paper describes the challenge in Japan for the application and mass production of nanofiber, which have been receiving so much attention recently.
2. Melt electrospinning
Electrospinning equipment of the solvent-free melting method has been receiving a considerable amount of attention, and research on electrospinning using lasers is detailed in the report of Ogata et al. [2−4] of Fukui University and Ohkoshi et al. [5−7] of Shinshu University. Here, the research of Dalton et al.  is introduced. Diameter of the fiber produced through the melt electrospinning only from polypropylene resin (PP-15, Bayer AG, MFI 15 cm3/10 min (230°C/2.16 kg)) were 35.6 μm. However, through the addition of the polypropylene modifier IRGATEC CR76 (Ciba-Geigy) to 1.5% in the solution, the fiber diameter decreased to 840 nm. This modifier is radical generator agent which controls a decrease in molecular weight of the polypropylene resin.
This is used to produce melt-blow, non-woven fabric using spun-bound grade resin, and improves the property of the barrier and the mechanical characteristic for the obtained nonwoven fibers.This additive has the possibility of thinning the fiber diameter by lowering the viscosity of the resin, however, it has also the possibility of polymer chain breakage.
Moreover, the melt electrospinning of the blend of polycaprolactone PCL (The molecular weight was 67000 g/mol) and copolymer PEG47-b-PCL95 of polyethylene glycol PEG and PCL were examined. Melt electrospinning becomes possible by blending the copolymer in PCL. Melt electrospun nanofiber was able to produce a thin fiber diameter by curbing the amount of discharge to 0.05 ml/h. The authors tried a further experiment using the general- purpose melt spinning equipment. In the melt electrospinning of low molecular weight PP, a fiber diameter of 1-5 μm was obtained (Fig. 1).
Research into the melt blow was carried out by Ellison et al. . A fiber averaging 300 nm was obtained by adjusting the melt temperature, blow temperature, and gas velocity along with the quantity of delivery using melt-blow grade PP (isotactic PP3746G, Exxon; MFR 1500 (230°C), Mn: 10600, Mw: 59000). The distribution of the fiber diameter varied from 100 to 2000 nm. Because melting time was as long as 30 min, however, Mn and Mw decreased to 38% and
Corresponding author: E-mail: firstname.lastname@example.org, Tel/Fax: +81-749-28-8582
d_p199_205_08-26RE.qxd 08.12.5 2:06 PM ページ 199
51%, respectively. Ellison asserted that in order to attain nanofiber with the melt-blow technique, it is crucial to have elasticity such that the fiber would not be severed through the friction by way of the blow process rather than the demanded the entanglement of the polymer chain.
3. Electronic material
Chi-Ching Kuo et al.  produced nanofiber with PMMA blended with various polyfluorenes (Fig. 2). The fibers obtained from the blending of PFTP/PMMA along with
PFO/PMMA, PFQ/PMMA, and PFBT/PMMA respectively showed the respective color luminescence of red, yellow, green, and blue. The luminescence efficiency exceeded that of spincasted film. The polyfluorenes were added to 1~50wt% in PMMA (with a molecular weight of 350000). The diameter of each nanofiber ranged from 250 to 750 nm. The dispersal of polyfluorene into the fiber occurs when the amount of additives is low, however, when the amount of polyfluorene is increased a core shell structure is formed to create a sequential aggregate structure in the center of the fiber. This aggregate structure showed a higher luminescence efficiency than that of spin-coated products.
Biomaterial is currently one of the most researched and utilized fields of nanofiber production. The nanofiber obtained by spinning from a 50-50 blend of chloroform fluid of PHB (poly (3-hydroxybutyrate), PHBV (poly (3- hydroxybutyrate-co-2-hydroxyvalerate)) excelled in adhesion and the cultivation of a cells in comparison to that obtained from cast film . The nanofiber mat from the 50-50 blend of w/w PHB/PHBV mixed solutions presented the highest ALP potency in these. These results signify the high potential for the use of these electrospinning nanofiber mats as bone-tissue scaffolds.
Santi Tungprapa et al.  compared various model medicines (naproxen (NAP), indometacin (IND), ibuprofen (IBU), sulindac (SUL) ) contained in calcium acetate (CA) nano fiber and their drug release characteristics with those of cast film. For each drug, a 20 wt% was added against the CA. The obtained nanofiber diameter was 263-297 nm. This nanofiber exhibited a quicker emission characteristic than cast film with all medicines.
Sakai et al.  proposed the scaffold of nanofiber through the electrospinning process. With the calcination of silica nano-nanofiber (50-800 nm) obtained by the electrospinning of tetraethoxysilane at 500°C as a starting material, they discovered that cells adhere to the fiber extremely effectively. It can be surmised that this is due to the improved adhesive properties between carrier and cell, because the various secreted proteins by the cells adhere more easily to the hydrophobic surface. Further, an MG63 osteoblast was cultured on silica nanofiber (uncalcinated). As a result, cells were cultivated along the distributed length of the fiber.
5. Manufacturing of nanofiber
5. 1 Present state of the world
Donaldson Co. Inc.  produces automobile oil filters by entrusting their manufacture to companies like E-spin 
Fig. 1 Melt electrospinning fiber of PP.
Fig. 2 Organic luminescence material .
d_p199_205_08-26RE.qxd 08.12.5 2:06 PM ページ 200
etc.. E-spin engages in the continuous production of non- woven nanofiber of a width of 64 inches. These are quite likely produced through the nozzle system. Finetex Technology Global (Hong Kong, Korea)  carries out the sale and processing on consignment of a products coated with nanofibers produced with electrospinning on nonwoven fabrics and products produced by sandwiching nanofiber between nonwoven fabric. Their factories are in Philippines. They have also decreased the nozzle system. Awa Paper MFG. Co. Ltd. (Japan) has been offering articles jointly developed with Finetex Technology in the market since August, 2008. As a filter medium for vehicle engines and gas turbines, it offers a product with a nanofiber coating on the filter paper surface. The nanofiber processing technology of a Finetex Technology was combined with technological know-how of the filter medium for engines from Awa paper MFG . With air filters, it is said that there is about a 50% improvement in ultra-fine, particle-capture performance such as the carbon dust and the double of durability were achieved in comparison with conventional filter mediums for the engines.
Nanotechnics (South Korea)  is a company in South Korea which Dupont purchased in 2002. Though they are developing nanofiber which excels in heat-resistance, it is not clear presently which specific products are employed. Nanostatics (USA)  was a venture-capital, nanofiber- processing company in Ohio, and it offered the coating of nanofiber through electrospinning through their proprietary technology. They are able to produce nanfibers of a width of 60 cm at a speed of 6 m per minute or more through fluid and electrostatic field control.
Furthermore, I.S. Kim of Shinshu University has developed a large-scale electrospinning device for trial purposes. It has produced nanofiber samples of a 60 cm width and 2 m length using a total of 65 (13 × 5 line) nozzles.
Hirose Paper Co. Ltd. [20, 21] has proposed a nanofiber production technique characterized by electrospinning through applying the voltage that maintains nanofiber conditions in bubbles that are continuously generated in a polymer solution (Fig. 3). Consequently, it is necessary to efficiently repeat the generation and bursting of the bubbles formed on the surface of the polymer solution. As an example of this process implementation, the degree of saponification for the polyvinyl alcohol is a mole percent of 87.0-89.0 dissolved to water, and the prepared concentration of the polymeric solution is 20